1 Macroporous ion-exchange membrane adsorbers: correlation between membrane structure, separation conditions and performance in bioseparation Makroporöse Ionenaustausch-Membranadsorber: Korrelation zwischen Membranstruktur, Trennbedingungen und Trennleistung in der Bioseparation Dissertation Zur Erlangung des akademischen Grades Dr. rer. nat. des Fachbereichs Chemie der Universität Duisburg-Essen vorgelegt von Dipl.-Ing. Jun Wang aus Shandong Essen 2009
2 Tag der mündlichen Prüfung: 15. September 2009 Vorsitzender: Prof. Dr. E. Hasselbrink Referent: Prof. Dr. M. Ulbricht Korreferent: Prof. Dr. T. Schmidt
3 Abstract In the first part of this dissertation, commercial Sartobind porous cation exchanger membranes, based on stabilized regenerated cellulose and with sulfonic acid (S) or carboxylic acid groups (C), were analyzed with respect to their pore structure in dry, slightly swollen and wet state by three microscopic methods, conventional scanning electron microscopy (SEM), environmental SEM (ESEM), and confocal laser scanning microscopy (CLSM). The dehydration behaviour of the membranes was in situ observed at varied vapour pressure in the chamber of the ESEM, indicating some deformations of the macropore structure (largest pore diameters up to 20 µm) and significant changes in dimension and mobility of smaller cellulose fibers within these macropores, both as function of water content of the membrane. The binding of mono-cy5-labelled lysozyme inside fluoresceine-labelled and unlabelled Sartobind membranes was monitored by CLSM. The characteristic fluorescence intensity distributions in areas of (146 * 146) µm 2 indicated that protein binding takes place predominately in a layer which is anchored to a fine cellulose fiber network and, to a lower degree, directly to thick cellulose fibers. Due to the limited thickness of this binding layer, a significant fraction of the macropores remained free of protein. Protein binding as function of concentration and incubation times was also monitored by CLSM and discussed related to the binding isotherms for the membranes Sartobind S and C. Further, a flow-through cell for the in situ monitoring with CLSM of protein binding during the binding step was built, and the results obtained for binding of lysozyme in membranes Sartobind S indicate that this experiment can give very important information on the dynamic behavior of porous membrane adsorbers during separation: The lateral microscopic resolution in the x,y plane enables the identification of different breakthrough times as function of the location (pore structure), and this information can help to explain possible reasons for axial dispersion (in z- direction) observed in breakthrough analyses of the same separation in a chromatography system. The combination of advanced microscopy with detailed investigations of static and dynamic protein binding will provide a better understanding of the coupling between mass transfer and reversible binding in membrane adsorbers onto separation performance, and it will provide valuable guide-lines for the development of improved membrane adsorbers. Based on the knowledge of the first part, new membrane adsorbers with carboxyl groups were prepared via UV-initiated heterogeneous grafting polymerization on Hydrosart macroporous regenerated cellulose membranes. The dynamic performance was investigated in detail with respect to the pore size and pore size distribution of the base membranes, ion-exchange
4 capacity, target proteins and architecture of the functional layers. Main characterization methods were pore analysis (BET and permporometry), titration, analysis of protein binding under static conditions including visualization by CLSM and chromatographic analysis of dynamic protein binding and system dispersion. The trade-off between ion-exchange capacity, permeability and static binding capacity of the functional membrane has partially been overcome by adapted architecture of the grafted functional layer achieved by the introduction of suited uncharged groups and stabilization of binding layer by chemical cross-linking. These membranes have negligible effect of flow rate. There is no considerable size exclusion effect for large proteins due to mesh size of functional cross-linked layers. Investigation of system dispersion based on breakthrough curves confirms that the adapted grafted layer architecture has drastically reduced the contribution of the membrane to total system dispersion. The optimum pore structure of base membranes in combination with the best suited architecture of functional layers was identified in this study. In the last part, the internal flow distribution of the flat sheet membrane modules was further quantified characterized based on a novel radial zone rate model. The proposed model partitioned the total void volume of the chromatography module into zones that have approximately homogeneous velocity profiles over time. The model was mathematically represented and analytically solved as a network of continuously stirred tank reactors (CSTR). An additional plug flow reactor (PFR) was connected in series with the CSTR network in order to account for a time-lag that was not associated with system dispersion. The capability of the model to describe experimental breakthrough data was compared to the often applied standard model for extra-membrane system dispersion which consists of a single CSTR in series with a PFR. The commercial CIM module and a custom designed Sartorius cell were studied with acetone and lysozyme as test tracers at varied flow rates and for varied membrane pore sizes under non-binding conditions. In all studied cases the proposed model fits the measured breakthrough curves better than the standard model. Moreover, the minimal number of radial flow zones that were required to accurately describe the observed breakthrough curves and the estimated flow fractions through these zones provided valuable information for the analysis and optimization of internal module designs.
5 This work was performed during the period from May 2006 to May 2009 at the Institute of Technical Chemistry (Lehrstuhl für Technische Chemie II), Department of Chemistry, Universität Duisburg-Essen, under the supervision of Prof. Dr. Mathias Ulbricht. I declare that this dissertation represents my own work, except where due acknowledgement is made. Jun Wang
6 Acknowledgement First I am deeply grateful to Prof. Dr. Mathias Ulbricht, who enables me to work at the group of Technische Chemie II, Uni Duisburg-Essen (UDE), and his constructive suggestions and active discussions during my work. Additionally, I would to express my respect for his respectable personality. I am very thankful to Prof. Dr. Torsten Schmidt, who acted as referee for this thesis. Dr. Rene Faber and Dr. Volkmar Thom from Sartorius Stedium Biotech GmbH, Göttingen have provided me the opportunity involved in this work, and given me their technical supports, active discussion during this work. And I would like to express my gratitude to everyone involved in my work: Dipl.-Biol. Florian Dismer and Prof. Dr. Jügen Hubbuch, Dr. Eric von Lieres from Institut für Biotechnologie of Jülich Research Center, Dipl.-Chem. Diana Spettmann and Prof. Hans-Curt Flemming from Biofilm Center of UDE, Dipl.-Ing. Smail Boukercha, Ms. Suhyoun Yu, Ms. Yu Feng from UDE. for their kindly co-operation work and technical support. The skilled technical support for the manufacture of the flow-through membrane module by Frank Matthes of UDE, is also acknowledged. I am very sorry for his suddenly young dead. MSc. Haofei Guo has kindly corrected some part of text of this work. I am very happy with the nice work atmosphere in the group of Technische Chemie II of UDE during the research work, special thanks go to Dipl.-Ing.Chem. Inge Danielzik, Ms. Claudia Schenk, Ms. Roswitha Nordmann-Silberg, MSc. Haofei Guo, Dr. Dongming He, Dr. Heru Sussanto, Dr. Qian Yang. Finally, I would like to thank all of my family - my parents, parents in law, and my daughter Tiantian, for their love and moral stimulation, especially, my husband Jionglu, who gives me the harbor of happiness.
7 This thesis is dedicated to my family for their love and moral stimulation
8 The main parts of this thesis have been published (submitted) in the following publications: 1. von Lieres, E., Wang, J., Ulbricht, M. Model based quantification of internal flow distributions from breakthrough curves of coin-shaped membrane chromatography modules, Ind. Eng. Chem. Res., 2009, submitted. 2. Wang, J., Faber, R., Ulbricht, M. Influence of pore structure and architecture of photo-grafted functional layers on separation performance of cellulose-based macroporous membrane adsorbers, J. Chromatogr. A, 2009, under reversion. 3. Wang, J., Dismer, F., Hubbuch, J., Ulbricht, M. Detailed analysis of membrane adsorber pore structure and protein binding by advanced microscopy, J. Membr. Sci., 320 (2008) 456.
9 Content 1. Introduction Background Principles of bioseparation Modes of preparative chromatography Membrane separation in bioprocesses Binding and mass transport phenomena of membrane adsorbers Equilibrium thermodynamics Principles of mass transport, fluid dynamics Advantages and limitations of membrane adsorbers Surface grafting techniques for polymeric membranes Photo-grafting functionalization on polymeric membranes via heterogeneous graft copolymerization for membrane adsorbers Characterization methods for membrane adsorbers Insights into the mathematical modeling of membrane adsorbers Conventional dispersion model Radial multi-zone flow model for system dispersion Modeling dynamic adsorption Problems and objectives Experiments Materials Characterization of membranes Microscopic methods Methods for SEM and measuring of wet samples using ESEM Membrane dehydration / hydration investigations Visualization of membrane morphology and protein binding by means of CLSM Characterization of membrane structure Membrane pore size distribution Membrane specific surface area Buffer permeability of membranes Determination of ion-exchange capacity Total ion-exchange capacity by titration method Dynamic ion-exchange capacity of membrane adsorber via ph transition. 46 I
10 Static and dynamic protein capacity Static binding capacity and protein binding isotherms Breakthrough curves and dynamic binding capacity Synthesis of cation-exchange membrane adsorbers via UV-initiated graft copolymerization Quantification of internal flow distribution of membrane modules based on zone rate modeling Results Characterization of commercial membrane adsorbers Protein binding equilibrium of commercial membrane adsorbers Detailed analysis of membrane adsorber pore structure and protein binding by advanced microscopy Membrane morphology Membrane hydration/dehydration Batch protein binding and static visualization of protein binding by CLSM In situ monitoring of protein binding under flow through by CLSM Preparation and characterization of novel membrane adsorbers Membrane pore structure and permeability Degree of grafting Variation of grafted layer structure Cation-exchange capacity Equilibrium behavior and static binding capacity Breakthrough curve and dispersion property Dynamic binding capacity Utilization of the membrane binding capacity under dynamic conditions Influence of the protein size Influence of the flow rate Static visualization of protein binding to modified membranes by CLSM Efficiency comparison of membrane modules Performance of dynamic binding capacity in different membrane modules Model based quantitative characterization of the internal flow distribution within membrane modules Discussion II
11 6.1. Detailed analysis of membrane adsorber pore structure and protein binding by advanced microscopy Images comparison Static visualization of protein binding by CLSM Protein binding under flow-through and in situ monitoring by CLSM Limitation of the used microscopic methods Influence of pore structure and architecture of photo-grafted functional layers on separation performance Base membrane Grafted functional polymer layers by UV-initiated grafting Influence of internal architecture of grafted functional layers Ion exchange capacity Membrane permeability and static binding capacity Influence of salt concentration on the grafted polymer architecture Dynamic membrane performance Comparison of protein binding capacity and other membrane adsorber system Effect of membrane module design on the efficiency of membrane adsorber process Conclusion and outlook Appendix A. References B. List of abbreviations C. List of publications and conferences D. Curriculum Vitae III
12 1. Introduction 1. Introduction With the increasing importance of biopharmaceutical therapeutics such as recombinant proteins, monoclonal antibodies, viral vaccines and plasmid DNA, bio-manufacturing industry has been boosted in the last years. The commercial manufacture requires a reliable process with high yield and high purity, and, most important, cost efficiency. Economic modeling of processes has shown that up to 80% of the overall costs are incurred during downstream purification process (1). Chromatography is widely employed at all operation stages of purification ranging from capture to polishing step. Conventional ion-exchange chromatographic steps are commonly based on resin bead packed columns (particles, typically having a diameter of >50 µm) with high resolution and high binding capacity. Generally those columns have low throughput and an oversized diameter is used to enable high volumetric rates in order to meet the requirement of process throughput. With the rapid improvements in upstream production, the traditional chromatographic platform has become the bottleneck in downstream process (2-6). The use of chromatographic membrane adsorbers has successfully overcome this problem in lab scale (7) and large scale (2, 8, 9). Chromatographic membrane adsorbers are based on macroporous supports from established membrane formation process technology. Subsequent chemical modification (6, 10-12) is performed for the attachment of functional groups acting as binding sites throughout the membrane. They were introduced as stationary phase in liquid chromatography separations since 1990s (13-16). Diverse research of membrane adsorbers has been performed towards more suitable and efficient base membranes (17-19), improved surface chemistries (20-25), optimized flow distribution of membrane devices in lab (26-28) and production scale (8, 29, 30) as well as mass transport phenomena (31-34). Membrane adsorber has been reported as a technology potentially suited for large-scale application due to its ability to integrate capture and purification steps for processing large amounts of product in relatively short times (35). Ion-exchange membrane chromatography has become the most successful application type of this technique (36-38). Membrane adsorbers combine the selectivity of chromatography resins with the high productivity of filtration membranes (4, 9, 10, 36). The key advantages of membrane adsorbers in comparison with conventional resin based porous adsorbers result from the pore structure of the membrane which allows a directional convective flow through the majority of the pores. The continuous character of membrane layer enables a simple scale-up and also 1
13 1. Introduction operation in a low range of trans-membrane pressure due to a relatively short effective thickness of the membrane layers. This membrane process allows high throughput with significant reduction in buffer consumption. Furthermore, the development of disposable membrane adsorber unit facilities the integration of these materials in bioprocesses, by saving cleaning and validation costs. They have been successfully applied for removing of trace impurities and potential contaminants in flow-through mode and for separation of sensitive bio-molecules such as blood factors, monoclonal antibodies, or technical enzymes where a rapid operation decreases the probability of their degradation (7, 9, 30). They are very useful for separation of large solutes such as DNA, RNA and viruses with molecular weight of over 250 kda in bind-and-elute mode (39-41). In large-scale recombinant monoclonal antibody production, flow-through anion exchange chromatography has been implemented for removing of a variety of viruses, DNA and endotoxin in capture and polish steps (42-44). However, lower surface-to-bed volume ratios generated lower binding capacity of membrane adsorber and inefficient flow distributions of membrane modules remain a challenge for wide routine application in process-scale productions (30, 45). Photo-initiated heterogeneous polymerization has been successfully applied as an easy and robust approach for the preparation of high capacity ion-exchange membrane adsorbers based on polypropylene and regenerated cellulose membranes (20, 22, 46, 47). Regenerated cellulose membrane is widely used in biotechnology due to its abundant availability, less binding capacity with protein and compatibility with biological systems. A systematic investigation of ion-exchange membrane adsorbers, prepared via photo-initiated heterogeneous polymerization, in terms of the correlations among properties of base membrane, functional layer via chemical functionalization as well as separation conditions (i.e. properties of liquid phase, flow rate, membrane module) should be prerequisite for better understanding of mass transfer and binding kinetic of membrane chromatography process. 2
14 2. Background 2. Background 2.1. Principles of bioseparation Bioseparation refers to the extraction and purification segment of a bioprocess. It is also termed as downstream purification process in fermentation technology (48). With the growing importance of biopharmaceutical therapeutics in treating human disease such as cancer, bioseparation is getting attractive in the manufacture of e.g. recombinant monoclonal antibodies, viral vaccines, and plasmid DNA (9, 39). Most important, it represents a major manufacturing cost for a wide variety of products. In a typical process train for the manufacture of monoclonal antoibodies (3) illustrated in Figure 2-1, this usually involves a native or recombinant protein A capture step combined with a cation exchange column for intermediate purification and an anion exchange column operating in flow through mode to remove negatively charged impurities such as DNA, host cell protein, endotoxins, and endogenous virus. Cell removal/clarification Step before the first chromatographic step: removement of cells and fine particels Affinity chromatography Capture step: volume reduction, major purification Virus-clearance Low ph-activiation, focus on enveloped virus Cation exchange chromatography Anion exchange adsorber Intermediate purification: removal of aggregates, DNA, HCP Polishing step(flow through): removal of DNA, HCP, Protein A, Endotoxin Virus-clearance Removal/inactivition, focus on non-enveloped virus Ultra-/Diafiltration Buffer exchange, concentration, formulation Figure 2-1. Typical process train for the manufacture of monoclonal antibodies 3
15 2. Background The biological activity of a protein is determined by its unique 3D-dimensional structure and surface functionality. Proteins are biopolymers formed by a linear sequence of the 20 natural occurring amino acids. The conformation is stabilized primarily by hydrophobic interactions due to the unfavourable free energy associated with solvation of non-polar groups in water. The net result is that the non-polar side chains tend to collapse together to form the hydrophobic core of protein. Hydrogen bonds between donor groups such a N-H and acceptor groups such as C=O with lone pair electrons stabilize the protein s secondary structure including α-helices and β-sheets. Positively charged amino groups and negatively charged carboxylic groups are typically located alone the protein exterior. The net protein charge is determined by the number and pka of these acidic and basic amino acids. The isoelectric point (pi) is the ph value at which the protein has no net electrical charge, typically determined by the equilibrium position in an isoelectric focusing gel or the lack of motion in an applied electric field (49). Bioseparation is largely based on chemical separation process. Some of the attributes of bioseparation distinguish it from chemical separation. For instance, biological products are commonly present in very low concentration in the being purified solution. The concentration of monoclonal antibodies is typically 0.1 mg/ml in the mammalian cell culture supernatants. Large volumes of dilute product streams have to be processed for gaining possible modest amounts of pure products. Hence a high throughput is required. Many impurities such as viruses, DNA and endotoxin and by-products exist in cell culture supernatant, and these impurities or by-products have similar chemical and physical properties to those of the target product. Biological products are thermolabile and susceptible to denaturation. Frequently, bioseparation is based on multi-technique separation based on one or more of the following factors (50): Molecular size using filtration, membrane separation, centrifugation, chromatography Density using centrifugation, sedimentation, flotation Diffusivity using centrifugation, filtration, sedimentation Polarity using extraction, chromatography, adsorption Solubility using extraction, precipitation, crystallization Electrostatic charge using adsorption, membrane separation, electrophoresis Volatility using distillation, membrane distillation, pervaporation 4
16 2.2. Modes of preparative chromatography 2. Background The binding of a dissolved protein to an immobilized ligand is due to one or several of the following interactions (51): 1. ion-ion or ion-dipole bonds 2. Hydrogen bonding 3. Hydrophobic interactions 4. Dispersion or van der Waals forces 5. Aromatic or Π-Π interactions Depending on the types of interactions involved, separation mechanism of chromatography can be classified into affinity chromatography, ion-exchange chromatography, hydrophobic interaction chromatography, reverse-phase chromatography, immobilized metal affinity chromatography and other types of chromatography such as size exclusion chromatography (52, 53). Affinity chromatography (AFC) ACF takes advantage of biological interactions to effect binding of specific solutes. Antibodies, antigens, or dyes are conjugated to polymer resins or membranes for purpose of binding specific solutes from a mixture. In particular, it deals with bio-specific affinity chromatography. The high affinities of protein for specific metals are used. Diversities of affinity chromatography have been used in bioprocess. For instance, the most widely utilized Protein A affinity chromatography for large-scale antibody separation, or the dye ligand chromatography such as Cibacron blue, which is through to mimic the nucleotide binding sites of enzyme. Immunoaffinity chromatography utilizes the high specificity and strength with antibodies bind to their antigens. Biomimetic ligands mimic the interactions of biomolecules with their natural ligands. For the immobilized metal ion affinity chromatography, the binding is to residues that are distributed over the protein surface (37, 51). 5
17 2. Background Ion-exchange chromatography (IEC) IEC is one of the most often used modes of chromatography for protein separation. This is due to the high dynamic capacities, high resolution and low relative costs of the IEC materials, and simple buffer used in large scale protein purification process (54). Another advantage of this technique is that the elution takes place under mild conditions so that the proteins maintain their native configuration during the chromatographic processing. Ion exchangers exploit surface charges on the protein under a given ph and salt ion concentration and interact with the protein predominately by electrostatic interactions (55). Elution is performed with increasing of salt concentration resulting in weakening of the ionic forces. Ion exchangers can be positively charged (strong, weak anion exchanger) or negatively charged (strong, weak cation exchanger) depending on the permanence of charge over a broad ph range. Commonly, strong exchanger can maintain their charge over a broader ph range than weak ion exchanger. A number of different functional groups are used. Most common are amines in the anion exchangers and the carboxylic acids in the cation exchangers. Strong anion exchangers have quaternary amines where strong cation exchangers have sulfonates (51). Hydrophobic interaction chromatography (HIC) and reverse phase chromatography (RPC) HIC and RPC are separations based on the attraction between hydrophobic groups on the protein and a hydrophobic matrix. In reverse phase chromatography, the sample is applied in an aqueous buffer and eluted in an organic buffer. The retention of protein on a reversed phase chromatography matrix is dependent on the relative hydrophobicity of the protein compared to the polarity of the fluid and solid phase. Elution occurs when the relative hydrophobicity of the protein is decreased by either decreasing the polarity of the fluid phase or increasing the polarity of the protein through the addition of an ion-pairing agent. In hydrophobic interaction chromatography the sample is applied under conditions of high salt concentration and eluted under conditions of low salt concentration. The mechanisms of partitioning of hydrophobic interaction chromatography can be explained in the same way as the interaction between non-polar solutes in water. Dissolving a non-polar substance in water is thermodynamically unfavorable. A non-polar solute forces the water to form a cavity in which the solute fits leading to a negative change in entropy. As the concentration of salts increases, the protein aggregate on the surface of adsorbents. HIC is sensible to used salt, ph, 6
18 buffer type and temperature. 2. Background Size exclusion chromatography (SEC) SEC is also called gel filtration. It separates solutes on the basis of their size. Molecules larger than the largest pores in the gel can not enter the gel and are eluted first. Smaller molecules enter the gel to varying extents, depending on their size and shape, and thus are retarded on their passage through the bed. In general, SEC resins (or matrixes) are hydrophilic polymer gels with a broad distribution of pore size. SEC is especially suitable for changing buffers, or for removing small molecules from protein solutions Membrane separation in bioprocesses Membranes are used extensively throughout the production, purification, and formulation of biotechnology products. The membrane can remove large impurities and pass the product, or retain the product and pass solvent and salts. The greatest interests have been in the application of pressure-driven processes of ultrafiltration, microfiltration, and virus filtration (36, 56). Microfiltration membranes are capable for removing particles larger than 0.1 µm. Ultrafiltration membranes are used for concentrating and diafiltering soluble macromolecules that have a size in solution of less than 0.1 µm. Membrane adsorber has been used as a technology potentially suitable for large-scale applications due to its ability to integrate capture and purification steps for processing large amounts of products in relatively short time. Current application of membrane adsorber is focusing on the aspects of two areas: flowthrough application aimed at removing trace impurities, such as virus, bind-elute purification of extremely large molecules essentially excluded from the internal pore structure of commercially available bead-based resins such as large molecule bind-elute purification include viral vectors, plasmids as well as extremely large protein molecules (MW >250 kda) (40). The flow velocity independency of membrane adsorber makes it ideally suitable for the purification of very large molecules such as plasmids or rotavirus like particles for gene therapy applications (39-41, 57). Membrane adsorbers are commercially available in variety of chemistries ranging from standard strong and weak anion and cation exchangers to hydrophobic interaction, reverse phase and affinity chemistries (4, 5). Membrane adsorber devices are available as stacked flat sheet in flow through or radial flow type, pleated as well as hollow fibers devices (4). 7
19 2. Background Currently commercially available membrane adsorbers are Sartorius s Sartobind family with a nominal pore size of 3 µm cellulosic membrane (58) and Pall s Mustang family with a nominal pore size of 0.8 µm polyethersulfone membrane (59). Polymeric monoliths made by a different manufacturing technology but having similar pore morphology compete with macroporous membrane adsorber, especially for ultrafast high resolution separation (60, 61) Binding and mass transport phenomena of membrane adsorbers Chromatography is a solute fractionation technique which relies on the dynamic distribution of molecules to be separated between a stationary phase and a mobile phase. The stationary phase can be packed particles in column or (stacked flat sheet) membranes in device. The mobile phase is passed through the device, typically at a fixed velocity. A pulse of sample containing the molecules to be separated is injected into the device along with the mobile phase. The moving velocity of molecules through the device depends on their respective interactions with the stationary phase (50). A chromatogram is influenced by several factors, such as the fluid dynamics inside the packed bed, mass transfer phenomena, and most importantly, the equilibrium of the adsorption. The elution profile of an ideal chromatogram depends only on the thermodynamic behavior of the chromatographic system. Real chromatograms take into account the additional kinetic of mass transfer and flow distribution Equilibrium thermodynamics The adsorption equilibrium is determined by the isotherm, which gives the correlation between the loading of the solutes on the adsorbent at different fluid phase concentration. Langmuir adsorption isotherm is the most common type of isotherm used in preparative chromatography. It describes quantitatively the build up of a layer of molecules on an adsorbent surface as a function of the concentration of the solute in the liquid in which it is in contact. For Langmuir isotherm, it is assumed that for a homogeneous surface, solute is bound in single layer and there are no lateral interferences between the adsorbed molecules. Assuming that the membrane has a fixed number of adsorption sites, S, to which the sample protein molecules, P, can bind reversibly in a monolayer pattern P + S ka kd PS (2-1) 8
20 2. Background Where PS represents protein-adsorbent. Equation (2-1) is associated to a reversible secondorder rate expression that can be written as: q t = ka * c *( qmax q) kd * q (2-2) at equilibrium, equation (2-2) reduces to Langmuir isotherm for single component: qmax * K * c q = (2-3) 1+ K * c with k k d K = Langmuir constant a Where ka and kd are respective association and dissociation rate constant. q is adsorbed amount on the membrane, c is protein concentration in bulk solution and q max maximal binding capacity of membrane. In the simplest case the adsorption isotherm is of the Langmuir type with a steep slope at the initial part and reaching a saturation value at higher amounts of adsorbed solute. The slope of the isotherm corresponds to the distribution (equilibrium) coefficient K, discriminating two parts of the isotherm: the linear and nonlinear parts. In the linear range K is equal to the Henry constant. Figure 2-2 Indicates the relationship of two different components and the related selectivity, which is devoted by Henry coefficient of the respective component in diluted solution. The j-component has higher affinity than i-component. For the nonlinear part K becomes smaller and reaches a limiting value at high solute concentrations. The subsequent part of the isotherm is called the overload regime whereas the linear part corresponds to the non-overloaded regime. Good resolution in the nonlinear range of the adsorption isotherm has to be achieved in terms of loading. In the preparative chromatography, column is operated under the overload conditions to achieve a high productivity, however purity of the product is thus limited. In addition, pressure drop should be as low as possible to allow operation at maximum linear velocity (62). 9